Hf-based high-k materials for Si nanocrystal floating gate memories
© Khomenkova et al; licensee Springer. 2011
Received: 23 September 2010
Accepted: 24 February 2011
Published: 24 February 2011
Pure and Si-rich HfO2 layers fabricated by radio frequency sputtering were utilized as alternative tunnel oxide layers for high-k/Si-nanocrystals-SiO2/SiO2 memory structures. The effect of Si incorporation on the properties of Hf-based tunnel layer was investigated. The Si-rich SiO2 active layers were used as charge storage layers, and their properties were studied versus deposition conditions and annealing treatment. The capacitance-voltage measurements were performed to study the charge trapping characteristics of these structures. It was shown that with specific deposition conditions and annealing treatment, a large memory window of about 6.8 V is achievable at a sweeping voltage of ± 6 V, indicating the utility of these stack structures for low-operating-voltage nonvolatile memory devices.
In recent years, nanocrystal-based memory devices have attracted considerable attention as a possible solution to overcome the scaling issue of electronic nonvolatile memories (NVMs) http://public.itrs.net/. By using discrete nanocrystals instead of the conventional continuous floating gate as charge storage nodes, local-defect-related leakage can be reduced efficiently to improve data retention . In this regard, discrete-trap type semiconductor storage materials such as Si and Ge nanocrystals (Si- and Ge-ncs) embedded in a dielectric matrix have been demonstrated as potential candidates for the fabrication of high-speed, high-density, low-power-consuming, and nonvolatile memories [2–6]. Several approaches have been reported for nanocrystal formation in a dielectric matrix, such as chemical vapor deposition, molecular beam epitaxy, or sputtering. The main attention was devoted to two major ones, namely deposition in vacuum and ion beam synthesis, since they are also used in the semiconductor industry for other purposes other than nanocrystal fabrication. Another approach for the fabrication of Si-ncs is the radio frequency (RF) magnetron sputtering, as discussed previously [7–11]. The excess Si content in the layers can be obtained by several ways. One of them is the sputtering of two separated (pure Si and SiO2) targets [7, 8, 12] or one composed (SiO2 target topped by Si chips) target in pure argon plasma [7, 13, 14]. The other one is the reactive approach, which deals with the sputtering of pure SiO2 target in mixed argon-hydrogen plasma [9–11] or pure Si target in argon-oxygen mixture . The Si excess is controlled by varying the hydrogen [9–11] or oxygen flow rate  in the plasma. After subsequent high-temperature annealing, Si-ncs can be easily formed in these Si-rich SiO2 (SRSO) composite layers [7–15].
One of the major problems associated with the downscaling of device dimensions is the quantum tunneling limit of SiO2, conventionally used as a gate dielectric material in metal-oxide-semiconductor field-effect transistors. In recent studies, high-k gate dielectrics replaced the conventional SiO2 dielectric to be used as tunnel and control oxides in NVM devices, which allows for a thinner equivalent oxide thickness without sacrificing the nonvolatility [16–20]. Furthermore, the thicker physical thickness of the high-k dielectrics ensures good retention characteristics, while due to unique band asymmetry with Si, their lower electron barrier height allows for a larger tunneling current at low control gate voltage when the device operates in the programming regime [18, 20]. In this regard, Hf-based dielectrics can be of immense interest.
In this work, different high-k/SRSO/SiO2 memory structures were fabricated by RF magnetron sputtering. The high-k layers (pure and Si-rich HfO2) were used as alternative tunnel layers. At the beginning, the effect of the deposition conditions and postdeposition annealing treatment was investigated separately for high-k and SRSO layers to obtain the optimal fabrication conditions for each material. Subsequently, the different stack structures were fabricated, and their structural and electrical properties were analyzed versus annealing treatment.
The structures investigated in the present study were grown on p-Si (100) substrates (resistivity of approximately 15 Ω cm) by RF magnetron sputtering. Prior to deposition, the substrates were subjected to standard RCA cleaning, dipped in a diluted hydrofluoric solution (10%), dried in N2, and immediately transferred to the vacuum chamber of the deposition setup. Single HfO-based and SRSO layers were developed to find the optimal conditions for fabrication of p-Si/tunnel layer/charge storage layer/control layer stack memory structures.
Four-inch HfO2 (99.9%) and SiO2 (99.995%) targets were used as starting targets to grow high-k (HfO-based) and low-k (pure or Si-rich SiO2) layers, respectively. The HfO-based layer was grown by sputtering either pure HfO2 or composed HfO2 + Si targets. The different Si content in the high-k layers was achieved by the variation of the number of Si chips topped on HfO2 target. In this study, Si surface ratio was R Si = 6% or 12%. The RF power density applied on HfO2 cathode, the argon flow, and the total plasma pressure were 0.74 W/cm2, 1.5 standard cubic centimeters per minute (sccm), and 40 μbar, respectively. The substrate temperatures were 45°C, 100°C, and 400°C.
The pure or Si-rich SiO2 layers were grown in the same chamber by sputtering of SiO2 target using either standard or reactive approaches. The deposition of pure SiO2 layers was performed in pure argon plasma (standard approach) with argon flow of 3.2 sccm. The Si-rich SiO2 layers were fabricated by reactive approach. The SiO2 target was sputtered in the mixed argon-hydrogen plasma. The argon and hydrogen flows were kept at 1.6 and 5.0 sccm, respectively. The RF power density applied on SiO2 cathode and the total plasma pressure were 0.74 W/cm2 and 20 μbar, correspondingly, for both pure and Si-rich SiO2 layers. The substrate temperatures were 45°C, 100°C, and 400°C.
The deposition conditions, mentioned above, were also used for the fabrication of trilayer structures where (1) the tunnel layer is HfO-based material (either pure or Si-rich HfO2), (2) the charge storage layer is Si-rich SiO2, and (3) the control layer is SiO2 or HfO-based layer.
To study the effect of the postdeposition processing on the thermal stability of the high-k layers as well as on the formation of Si-ncs inside SiO2 ones, both single-layer and trilayer structures were annealed in a conventional furnace within the temperature range of 800°C to 1,100°C for 10 to 30 min under nitrogen flow. In some cases, an additional annealing in forming gas at 400°C for 60 min was also used to passivate dangling bonds, if any. After this, the Al contacts were deposited by means of thermal evaporation of Al target on the back and face sides of the structures, followed by an annealing of the final structures at 400°C for 20 min in forming gas flow.
The combination of different methods allows information about film properties to be obtained. Thus, infrared attenuated total reflectance (ATR) was used to study the structure and chemical composition of the films. ATR-FTIR spectra were measured in the range 600 to 4,000 cm-1 by means of a 60° Ge Smart Ark accessory inserted in a Thermo Nicolet spectrometer (Nexus model 670) (Thermo Nicolet Corporation, Madison, USA). X-ray diffraction ( XRD) data were obtained using a Phillips X'PERT PRO device http://www.panalytical.com/ with Cu Kα radiation (λ = 0.1514 nm) at a fixed grazing angle incidence of 0.5°. An asymmetric grazing geometry was chosen to increase the volume of material interacting with X-ray beam as well as to eliminate the contribution from Si substrate. The electrical properties of the samples were studied at different frequencies using an HP 4192A LF Impedance Analyzer http://www.home.agilent.com/.
Results and discussion
The fabrication of an NVM cell requires a perfect control of four main parameters: (1) the tunnel oxide thickness, (2) the nanocrystal density, (3) the nanocrystal diameter, and (4) the control oxide thickness. In these regards, properties of the samples were analyzed at different fabrication steps and applied to get an insight on the formation and quality of the structures. Prior to describing the electrical properties of the trilayer stack structures, let us consider separately the parameters of single pure and Si-rich HfO2 layers as well as Si-rich SiO2 layers.
HfO-based tunnel layers
In our previous study , the thermal stability of amorphous structure and the chemical composition of pure HfO 2 layers grown by RF magnetron sputtering after annealing at 800°C to 850°C for 15 min in nitrogen flow have been discussed in detail. Besides, the formation of monoclinic HfO2 phase after treatment at higher annealing temperature (T A = 900°C to 1,100°C) was also demonstrated. However, HfSiO layers were found to be stable at 950°C, whereas the increase of annealing temperature (T A) led to the formation of tetragonal HfO2 phase. The tetragonal phase is more preferred, since it has a higher dielectric constant (about 25). It was clearly demonstrated that the Si incorporation plays the major role for the improvement of the thermal stability of the HfO-based layers .
The high-frequency capacitance-voltage (C-V) study of metal-insulator-semiconductor (MIS) capacitors containing pure HfO2 layers (as-deposited as well as annealed at 800°C for 15 min) was performed for the samples grown at different temperatures. In most cases, the C-V curves of the annealed samples demonstrated less stretch-out effect compared to the as-deposited films due to lower number of interface states. However, the significant negative shift of flat-band voltage (V fb) up to -2 V indicates the existence of considerable amount of positive oxide charges in the films. The introduction of positive charges can be caused by the formation of SiO x interfacial layer between HfO2 layer and Si substrate as a result of oxygen diffusion towards Si wafer under annealing treatment . In addition, the presence of oxygen vacancies inside HfO2 films that is most common in high-k gate dielectrics also gives rise to positive charge .
One of the limiting factors for oxygen diffusion inside HfO2 films can be Si incorporation in HfO 2 -based layers. It was supposed that due to covalent nature of Si-O bonds, the formation of oxygen interstitials and vacancies will be prevented, which in turn can give rise to an improvement in the electrical properties of high-k materials. In this regard, the effect of the Si content on the electrical properties of our high-k films was investigated.
In contrast, HfSiO samples grown with R Si = 6% exhibit regular C-V curves. The extremely low hysteresis, along with a sharp transition from accumulation to depletion, demonstrates the high quality of interfacial as well as bulk properties of this layer.
We have further investigated the effect of deposition temperature on the C-V characteristics of HfSiO layers grown with R Si = 12%. As can be seen from Figure 1b, the samples deposited at higher temperature (T S = 400°C) show better C-V characteristics than their counterparts grown at T S = 45°C and 100°C. Therefore, we can conclude that higher deposition temperature is preferable for the Si-rich HfO2-based layers. Moreover, as one can see from Figure 1a, b, the C-V characteristics of HfSiO layer grown with R Si = 12% at T s = 400°C are similar to the case of HfSiO films grown at R Si = 6% and T s = 45°C. However, in the former case, the hysteresis effect is negligible compared to the last one. In this regard, one can deduce that the HfSiO layer grown with the R Si = 12% at T s = 400°C is more suitable for the fabrication of the structures even at high-temperature deposition, whereas the material with the lower Si content or pure ones can be used for low-temperature deposition approach.
Considering the above results, different types of the structures, such as HfO2/SRSO/HfO2(SiO2) and HfSiO/SRSO/HfSiO, were fabricated and their electrical properties were studied versus annealing treatment. Since SRSO single layers with embedded Si-ncs are considered as charge storage layers, they will be analyzed prior to describe the properties of the trilayer structures.
SRSO single layers
The most common method to form Si-ncs entails the deposition of a thick SRSO monolayer, in which the formation of Si-ncs occurs due to phase separation on Si and SiO2 stimulated by high-temperature annealing. The observation of the bright photoluminescence (PL) emission in the visible spectral range is the evidence of the presence of Si-ncs. Unfortunately, the size distribution of Si-ncs in composite SRSO layers is usually broad. Thus, for the fine control of Si-ncs size the multilayer (ML) approach, where SRSO layers are alternated by SiO2 ones, can be applied. In this case, the control of Si-ncs occurs by means of precise thickness for SRSO layer [11, 15]. In the present study, the [SRSO/SiO2] MLs were grown with the aim of obtaining optimal conditions for Si-ncs formation, which can be applied in future memory structures. Each ML contained 20 [SRSO/SiO2] periods. For all the stacks, the thickness of SiO2 layer was 3 nm, whereas the thickness of SRSO layer varied from 2 to 6 nm for different MLs.
It is worth to note that pure HfO2 material does not conserve amorphous structure upon an annealing at high temperatures (900°C to 1,100°C). Such treatment results in the formation of monoclinic HfO2 phase in the single layers . The appearance of grain boundaries can significantly degrade electrical properties of the structures. Thus, this dictates the elaboration of the lower thermal budget conditions for the formation of Si-ncs. In this regard, grown SRSO/SiO2 MLs were also annealed at relatively lower temperatures (800°C to 950°C) for 10 to 15 min. For all the cases, PL emission was obtained. However, the brightest light emission was found for [2-nm-SRSO/SiO2]20 ML structure (Figure 2b). Its PL spectrum is narrower than that observed for [6-nm-SRSO/SiO2]20 ML. It is obvious that the phase separation can occur easily for thinner SRSO layers due to smaller Si diffusion path, and this can explain the narrower PL band for [2-nm-SRSO/SiO2]20 ML, confirming the narrower size distribution of Si-ncs. The decomposition process usually completes faster for thinner SRSO layer, resulting in the formation of Si-ncs and SiO2 phase (instead of SiO x one). So, the formation of Si-ncs/SiO2 barrier instead of Si-ncs/SiO x is more probable for thinner layers. Additionally, such layers are more preferable for obtaining better electrical properties.
Based on the abovementioned results, the deposition and postdeposition conditions elaborated for single HfO-based layers and for SRSO/SiO2 MLs were adopted for the fabrication of trilayer structures, in which SRSO layer plays the role of charge storage layer. Low thermal budget was applied for the SRSO layers to form Si-ncs accompanied by the conservation of the amorphous nature of HfO-based layer.
The electrical properties of the structures
The trilayer structures with the fixed thicknesses of tunnel (4 nm) and control (10 nm) layers and different thicknesses of SRSO layer (from 2 to 4 nm) were studied versus annealing treatment. As it was shown above, for all of them, the formation of Si-ncs is expected upon annealing. Going further, it is worth to note that the best electrical properties were demonstrated by the structures with 2-nm-thick SRSO layers, and they will be discussed below.
The annealing temperature was further increased to 950°C (keeping the same annealing time as 15 min), and significant charge storage was achieved at relatively lower sweep voltages. The frequency dependent C-V curves were found to be almost constant within the frequency range of 1 MHz to 10 kHz. All of them show a sharp transition from accumulation to inversion region, indicating less number of interfacial traps. The memory window value increases from ΔV fb = 1 V to ΔV fb = 7 V with increasing the sweep voltage from ± 1 to ± 7 V. It is worth noting that with annealing temperature increasing from 800°C to 950°C, the ΔV fb value increases from 2.3 to 6.8 V at a sweep voltage of ± 6 V. This can be due to the increase of the Si-ncs number and to the better performance of surrounding SiO2 matrix. The latter favors the formation of the higher barrier for carrier tunneling from gate contact. However, annealing at T A > 950°C results in a decrease of ΔV fb value to 0.05 V (Figure 4f). This can be caused by complete oxidation of SRSO layer without formation of Si-ncs and by Si out-diffusion from the SRSO layer through the HfO2 layer [22, 23].
Considering the results presented above, the investigation of the structures by means of ATR and XRD methods was performed to obtain the information about transformation of SRSO layer as well as about the nature of HfO2 tunnel layer. In the last case, this was impacted by the fact that an annealing at temperatures higher than 800°C could not favor the stability of HfO2 amorphous structure. It is more probable that the crystallization of HfO2 layer occurred. However, the ATR spectra did not reveal any formation of monoclinic HfO2 phase, since HfO vibration band was found to be featureless. At the same time, the XRD study showed that at T A > 900°C, the formation of tetragonal HfO2 phase occurs, while at lower T A, the tunnel layer conserves its amorphous structure (not shown here). However, the determination of Si-ncs by this method met some difficulties due to overlapping of the peaks from tetragonal HfO2 phase and Si-ncs. The TEM observation of the abovementioned samples is currently under investigation to get a clear picture about the evolution of Si-ncs and HfO2 layers. However, we can conclude that for T A = 950°C, the memory effect is predominantly due to Si-ncs formation.
The application of pure HfO2 and HfSiO layers fabricated by RF magnetron sputtering as alternative tunnel layers for high-k/Si-ncs-SiO2/SiO2 memory structures is demonstrated. The effect of the Si incorporation of the electrical properties of high-k layers was investigated. It is shown that there is an optimal Si content allowed to obtain desirable C-V parameters for single layers. The Si-rich SiO2 layers were used as charge storage layers, and their properties were studied versus deposition conditions and annealing treatment. The C-V measurements of fabricated stack structures show that with specific deposition conditions and annealing treatment, a large memory window (about 6.8 V) is achievable at a sweeping voltage of ± 6 V, indicating the utility of these stack structures for low-operating-voltage NVM devices.
This work is supported by the French National Research Agency (ANR) through the Nanoscience and Nanotechnology Program (NOMAD Project no. ANR-07-NANO-022-02) and, for one of the author (L.K.), by the Region Basse Normandie through the CPER project - Nanoscience axe (2007-2013).
- Aaron VY, Leburton JP: Flash memory: towards single-electronics. IEEE Potentials 2002, 21: 35. 10.1109/MP.2002.1044216View Article
- Tiwari S, Rana F, Hanafi H, Hartstein A, Crabbe EF, Chan K: A silicon nanocrystals based memory. Appl Phys Lett 1996, 68: 1377. 10.1063/1.116085View Article
- Hanafi HI, Tiwari S, Khan I: Fast and long retention-time nano-crystal memory. IEEE Trans Electron Devices 1996, 43: 1553. 10.1109/16.535349View Article
- King YC, King TJ, Hu C: Charge-trap memory device fabricated by oxidation of Si1-x Gex. IEEE Trans Electron Devices 2001, 48: 696. 10.1109/16.915694View Article
- Ng CY, Chen TP, Ding L, Fung S: Memory characteristics of MOSFETs with densely stacked silicon nanocrystal layers in the gate oxide synthesized by low-energy ion beam. IEEE Electron Device Lett 2006, 27: 231. 10.1109/LED.2006.871183View Article
- Kapetanakis E, Normand P, Tsoukalas D, Beltsios K, Stoemenos J, Zhang S, van der Berg J: Charge storage and interface states effects in Si-nanocrystal memory obtained using low-energy Si+ implantation and annealing. Appl Phys Lett 2000, 77: 3450. 10.1063/1.1328101View Article
- Khomenkova L, Korsunska N, Yukhimchuk V, Jumayev B, Torchynska T, Vivas Hernandez A, Many A, Goldstein Y, Savir E, Jedrzejewski J: Nature of visible luminescence and its excitation in Si-SiOx systems. Journal of Luminescence. J Lumin 2003, 102–103: 705. 10.1016/S0022-2313(02)00628-2View Article
- Baran M, Korsunska N, Khomenkova L, Stara T, Sheinkman M, Goldstein Y, Jedrzejewski J, Savir E: Investigation of Aging Process of Si-SiO(x) Structures with Silicon Quantum Dots. J Appl Phys 2005, 98: 113515. 10.1063/1.2134887View Article
- Gourbilleau F, Voivenel P, Portier X, Rizk R: A novel method for the deposition of Si-SiO2 superlattices. Microel Reliability 2000, 40: 889. 10.1016/S0026-2714(99)00334-0View Article
- Gourbilleau F, Portier X, Ternon C, Voivenel P, Rizk R: Si rich/SiO2 nanostructured multilayers by reactive magnetron sputtering. Appl Phys Lett 2001, 78: 3058. 10.1063/1.1371794View Article
- Portier X, Ternon C, Gourbilleau F, Dufour C, Rizk R: Anneal temperature dependence of Si-SiO2 superlattices photoluminescence. Physica E 2003, 16: 439. 10.1016/S1386-9477(02)00628-8View Article
- Hao XJ, Podhorodecki AP, Shen YS, Zatryb G, Misiewicz J, Green MA: Effects of Si-rich oxide layer stoichiometry on the structural and optical properties of Si QD/SiO2 multilayer films. Nanotechnology 2009, 20: 485703. 10.1088/0957-4484/20/48/485703View Article
- He Y, Bi L, Feng JY, Wu QL: Properties of Si-rich SiO2 films by RF magnetron sputtering. J Cryst Growth 2005, 280: 352. 10.1016/j.jcrysgro.2005.03.081View Article
- Seifarth H, Groetzschel R, Markwitz A, Matz W, Nitzsche P, Rebohle L: Preparation of SiO2 films with embedded Si nanocrystals by reactive r.f. magnetron sputtering. Thin Solid Films 1998, 330: 202. 10.1016/S0040-6090(98)00609-9View Article
- Tomozeiu N, van Hapert JJ, van Faassen EE, Arnoldbik W, Vredenberg AM, Habraken FHPM: Structural properties of a-SiOx layers deposited by reactive magnetron sputtering technique. J Optoelect Adv Mat 2002, 4: 513.
- Wan Q, Zhang NL, Liu WL, Lin CL, Wang TH: Memory and negative photoconductivity effects of Ge nanocrystals embedded in ZrO2/Al2O3 gate dielectrics. Appl Phys Lett 2003, 83: 138. 10.1063/1.1589196View Article
- Lu XB, Lee PF, Dai JY: Synthesis and memory effect study of Ge nanocrystals embedded in LaAlO3 high-k dielectrics. Appl Phys Lett 2005, 86: 203111. 10.1063/1.1926414View Article
- Kim DW, Kim T, Banerjee SK: Memory characterization of SiGe quantum dot flash memories with HfO2 and SiO2 tunneling dielectrics. IEEE Trans Electron Devices 2003, 50: 1823. 10.1109/TED.2003.815370View Article
- Chan MY, Lee PS, Ho V, Seng HL: Ge nanocrystals in lanthanide-based Lu2O3 high-k dielectric for nonvolatile memory applications. J Appl Phys 2007, 102: 094307. 10.1063/1.2803883View Article
- Lee JJ, Wang X, Bai W, Lu N, Kwong DL: Theoretical and experimental investigation of Si nanocrystal memory device with HfO2 high-k tunneling dielectric. IEEE Trans Electron Devices 2003, 50: 2067. 10.1109/TED.2003.816107View Article
- Khomenkova L, Dufour C, Coulon PE, Bonafos C, Gourbilleau F: High-k Hf-based layers grown by RF magnetron sputtering. Nanotechnology 2010, 21: 095704. 10.1088/0957-4484/21/9/095704View Article
- Foster AS, Lopez Gejo F, Shluger AL, Nieminen RM: Vacancy and interstitial defects in hafnia. Phys Rev B 2002, 65: 174117. 10.1103/PhysRevB.65.174117View Article
- Perego M, Seguini G, Wiemer C, Fanciulli M, Coulon PE, Bonafos C: Si nanocrystal synthesis in HfO2/SiO/HfO2 multilayer structures. Nanotechnology 2010, 21: 055606. 10.1088/0957-4484/21/5/055606View Article
- Chiang KH, Lu SW, Peng YH, Kuang CH, Tsai CS: Characterization and modeling of fast traps in thermal agglomerating germanium nanocrystal metal-oxide-semiconductor capacitor. J Appl Phys 2008, 104: 014506. 10.1063/1.2953194View Article
- Khomenkova L, Portier X, Cardin J, Gourbilleau F: Thermal stability of high-k Si-rich HfO2 layers grown by RF magnetron sputtering. Nanotechnology 2010, 21: 285707. 10.1088/0957-4484/21/28/285707View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.